#------------------------------------------------------------------------------
#$Date: 2016-03-26 02:38:45 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180149 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/46/7104684.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7104684
loop_
_publ_author_name
'Mathieu, Josiah L'
'Latturner, Susan E'
_publ_section_title
;
 Zintl phase as dopant source in the flux synthesis of
 Ba(1-x)K(x)Fe(2)As(2) type superconductors.
;
_journal_issue                   33
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              4965
_journal_page_last               4967
_journal_paper_doi               10.1039/b910749e
_journal_volume                  34
_journal_year                    2009
_chemical_formula_sum            'As2 Ba0.68 Fe2 K0.24 Sn0.07'
_chemical_formula_weight         372.59
_chemical_name_systematic
;
?
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   3.946(2)
_cell_length_b                   3.946(2)
_cell_length_c                   13.431(9)
_cell_measurement_reflns_used    125
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      32.39
_cell_measurement_theta_min      3.03
_cell_volume                     209.1(2)
_computing_cell_refinement       'Bruker APEX2'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker APEX2'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.887
_diffrn_measured_fraction_theta_max 0.887
_diffrn_measurement_device_type  'Bruker APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0261
_diffrn_reflns_av_sigmaI/netI    0.0220
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            609
_diffrn_reflns_theta_full        32.39
_diffrn_reflns_theta_max         32.39
_diffrn_reflns_theta_min         3.03
_exptl_absorpt_coefficient_mu    29.173
_exptl_absorpt_correction_T_max  0.747
_exptl_absorpt_correction_T_min  0.501
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'via SADABS (Bruker, 2000)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    5.935
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             310
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_refine_diff_density_max         2.118
_refine_diff_density_min         -1.681
_refine_diff_density_rms         0.235
_refine_ls_extinction_coef       0.0054(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.294
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     13
_refine_ls_number_reflns         125
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.288
_refine_ls_R_factor_all          0.0245
_refine_ls_R_factor_gt           0.0232
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0224P)²+1.2844P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0558
_refine_ls_wR_factor_ref         0.0563
_reflns_number_gt                117
_reflns_number_total             125
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b910749e.txt
_cod_data_source_block           'data_0m3'
_cod_original_sg_symbol_H-M      I4/mmm
_cod_database_code               7104684
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.0000 0.0000 0.0000 0.0167(4) Uani 0.683(8) 16 d SP . .
K1 K 0.0000 0.0000 0.0000 0.0167(4) Uani 0.244(10) 16 d SP . .
As2 As 0.0000 0.0000 0.35435(8) 0.0112(4) Uani 1 8 d S . .
Fe3 Fe 0.0000 0.5000 0.2500 0.0109(4) Uani 1 8 d S . .
Sn1 Sn 0.0000 0.0000 0.0903(16) 0.0167(4) Uani 0.037(2) 8 d SP . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Sn1 Ba1 Sn1 180.0 17 . ?
Sn1 Ba1 As2 125.03(3) 17 25 ?
Sn1 Ba1 As2 54.97(3) . 25 ?
Sn1 Ba1 As2 54.97(3) 17 9_444 ?
Sn1 Ba1 As2 125.03(3) . 9_444 ?
As2 Ba1 As2 180.00(3) 25 9_444 ?
Sn1 Ba1 As2 125.03(3) 17 25_455 ?
Sn1 Ba1 As2 54.97(3) . 25_455 ?
As2 Ba1 As2 70.76(3) 25 25_455 ?
As2 Ba1 As2 109.24(3) 9_444 25_455 ?
Sn1 Ba1 As2 125.03(3) 17 25_545 ?
Sn1 Ba1 As2 54.97(3) . 25_545 ?
As2 Ba1 As2 70.76(3) 25 25_545 ?
As2 Ba1 As2 109.24(3) 9_444 25_545 ?
As2 Ba1 As2 109.93(6) 25_455 25_545 ?
Sn1 Ba1 As2 54.97(3) 17 9_454 ?
Sn1 Ba1 As2 125.03(3) . 9_454 ?
As2 Ba1 As2 109.24(3) 25 9_454 ?
As2 Ba1 As2 70.76(3) 9_444 9_454 ?
As2 Ba1 As2 70.07(6) 25_455 9_454 ?
As2 Ba1 As2 180.00(3) 25_545 9_454 ?
Sn1 Ba1 As2 54.97(3) 17 9_544 ?
Sn1 Ba1 As2 125.03(3) . 9_544 ?
As2 Ba1 As2 109.24(3) 25 9_544 ?
As2 Ba1 As2 70.76(3) 9_444 9_544 ?
As2 Ba1 As2 180.00(3) 25_455 9_544 ?
As2 Ba1 As2 70.07(6) 25_545 9_544 ?
As2 Ba1 As2 109.93(6) 9_454 9_544 ?
Sn1 Ba1 As2 125.03(3) 17 25_445 ?
Sn1 Ba1 As2 54.97(3) . 25_445 ?
As2 Ba1 As2 109.93(6) 25 25_445 ?
As2 Ba1 As2 70.07(6) 9_444 25_445 ?
As2 Ba1 As2 70.76(3) 25_455 25_445 ?
As2 Ba1 As2 70.76(3) 25_545 25_445 ?
As2 Ba1 As2 109.24(3) 9_454 25_445 ?
As2 Ba1 As2 109.24(3) 9_544 25_445 ?
Sn1 Ba1 As2 54.97(3) 17 9_554 ?
Sn1 Ba1 As2 125.03(3) . 9_554 ?
As2 Ba1 As2 70.07(6) 25 9_554 ?
As2 Ba1 As2 109.93(6) 9_444 9_554 ?
As2 Ba1 As2 109.24(3) 25_455 9_554 ?
As2 Ba1 As2 109.24(3) 25_545 9_554 ?
As2 Ba1 As2 70.76(3) 9_454 9_554 ?
As2 Ba1 As2 70.76(3) 9_544 9_554 ?
As2 Ba1 As2 180.00(3) 25_445 9_554 ?
Sn1 Ba1 Fe3 149.56(2) 17 . ?
Sn1 Ba1 Fe3 30.44(2) . . ?
As2 Ba1 Fe3 37.977(17) 25 . ?
As2 Ba1 Fe3 142.023(17) 9_444 . ?
As2 Ba1 Fe3 37.977(17) 25_455 . ?
As2 Ba1 Fe3 78.37(4) 25_545 . ?
As2 Ba1 Fe3 101.63(4) 9_454 . ?
As2 Ba1 Fe3 142.023(17) 9_544 . ?
As2 Ba1 Fe3 78.37(4) 25_445 . ?
As2 Ba1 Fe3 101.63(4) 9_554 . ?
Sn1 Ba1 Fe3 149.56(2) 17 25 ?
Sn1 Ba1 Fe3 30.44(2) . 25 ?
As2 Ba1 Fe3 37.977(17) 25 25 ?
As2 Ba1 Fe3 142.023(17) 9_444 25 ?
As2 Ba1 Fe3 78.37(4) 25_455 25 ?
As2 Ba1 Fe3 37.977(17) 25_545 25 ?
As2 Ba1 Fe3 142.023(17) 9_454 25 ?
As2 Ba1 Fe3 101.63(4) 9_544 25 ?
As2 Ba1 Fe3 78.37(4) 25_445 25 ?
As2 Ba1 Fe3 101.63(4) 9_554 25 ?
Fe3 Ba1 Fe3 41.98(3) . 25 ?
Fe3 As2 Fe3 70.41(3) 25_455 1_545 ?
Fe3 As2 Fe3 109.22(6) 25_455 25 ?
Fe3 As2 Fe3 70.41(3) 1_545 25 ?
Fe3 As2 Fe3 70.41(3) 25_455 . ?
Fe3 As2 Fe3 109.22(6) 1_545 . ?
Fe3 As2 Fe3 70.41(3) 25 . ?
Fe3 As2 Sn1 134.9(2) 25_455 25 ?
Fe3 As2 Sn1 134.9(2) 1_545 25 ?
Fe3 As2 Sn1 65.9(3) 25 25 ?
Fe3 As2 Sn1 65.9(3) . 25 ?
Fe3 As2 Sn1 65.9(3) 25_455 25_445 ?
Fe3 As2 Sn1 65.9(3) 1_545 25_445 ?
Fe3 As2 Sn1 134.9(2) 25 25_445 ?
Fe3 As2 Sn1 134.9(2) . 25_445 ?
Sn1 As2 Sn1 150.2(8) 25 25_445 ?
Fe3 As2 Sn1 65.9(3) 25_455 25_455 ?
Fe3 As2 Sn1 134.9(2) 1_545 25_455 ?
Fe3 As2 Sn1 134.9(2) 25 25_455 ?
Fe3 As2 Sn1 65.9(3) . 25_455 ?
Sn1 As2 Sn1 86.2(2) 25 25_455 ?
Sn1 As2 Sn1 86.2(2) 25_445 25_455 ?
Fe3 As2 Sn1 134.9(2) 25_455 25_545 ?
Fe3 As2 Sn1 65.9(3) 1_545 25_545 ?
Fe3 As2 Sn1 65.9(3) 25 25_545 ?
Fe3 As2 Sn1 134.9(2) . 25_545 ?
Sn1 As2 Sn1 86.2(2) 25 25_545 ?
Sn1 As2 Sn1 86.2(2) 25_445 25_545 ?
Sn1 As2 Sn1 150.2(8) 25_455 25_545 ?
Fe3 As2 Ba1 143.558(11) 25_455 9 ?
Fe3 As2 Ba1 143.558(11) 1_545 9 ?
Fe3 As2 Ba1 81.98(4) 25 9 ?
Fe3 As2 Ba1 81.98(4) . 9 ?
Sn1 As2 Ba1 20.1(4) 25 9 ?
Sn1 As2 Ba1 130.0(4) 25_445 9 ?
Sn1 As2 Ba1 81.5(2) 25_455 9 ?
Sn1 As2 Ba1 81.5(2) 25_545 9 ?
Fe3 As2 K1 143.558(11) 25_455 9 ?
Fe3 As2 K1 143.558(11) 1_545 9 ?
Fe3 As2 K1 81.98(4) 25 9 ?
Fe3 As2 K1 81.98(4) . 9 ?
Sn1 As2 K1 20.1(4) 25 9 ?
Sn1 As2 K1 130.0(4) 25_445 9 ?
Sn1 As2 K1 81.5(2) 25_455 9 ?
Sn1 As2 K1 81.5(2) 25_545 9 ?
Ba1 As2 K1 0.0 9 9 ?
Fe3 As2 K1 143.558(11) 25_455 9_545 ?
Fe3 As2 K1 81.98(4) 1_545 9_545 ?
Fe3 As2 K1 81.98(4) 25 9_545 ?
Fe3 As2 K1 143.558(11) . 9_545 ?
Sn1 As2 K1 81.5(2) 25 9_545 ?
Sn1 As2 K1 81.5(2) 25_445 9_545 ?
Sn1 As2 K1 130.0(4) 25_455 9_545 ?
Sn1 As2 K1 20.1(4) 25_545 9_545 ?
Ba1 As2 K1 70.76(3) 9 9_545 ?
K1 As2 K1 70.76(3) 9 9_545 ?
Fe3 As2 Ba1 81.98(4) 25_455 9_455 ?
Fe3 As2 Ba1 143.558(11) 1_545 9_455 ?
Fe3 As2 Ba1 143.558(11) 25 9_455 ?
Fe3 As2 Ba1 81.98(4) . 9_455 ?
Sn1 As2 Ba1 81.5(2) 25 9_455 ?
Sn1 As2 Ba1 81.5(2) 25_445 9_455 ?
Sn1 As2 Ba1 20.1(4) 25_455 9_455 ?
Sn1 As2 Ba1 130.0(4) 25_545 9_455 ?
Ba1 As2 Ba1 70.76(3) 9 9_455 ?
K1 As2 Ba1 70.76(3) 9 9_455 ?
K1 As2 Ba1 109.93(6) 9_545 9_455 ?
As2 Fe3 As2 109.60(3) . 25_455 ?
As2 Fe3 As2 109.22(6) . 1_565 ?
As2 Fe3 As2 109.60(3) 25_455 1_565 ?
As2 Fe3 As2 109.60(3) . 25 ?
As2 Fe3 As2 109.22(6) 25_455 25 ?
As2 Fe3 As2 109.60(3) 1_565 25 ?
As2 Fe3 Fe3 125.203(16) . 25_565 ?
As2 Fe3 Fe3 125.202(16) 25_455 25_565 ?
As2 Fe3 Fe3 54.798(16) 1_565 25_565 ?
As2 Fe3 Fe3 54.798(16) 25 25_565 ?
As2 Fe3 Fe3 54.797(16) . 25_455 ?
As2 Fe3 Fe3 54.798(16) 25_455 25_455 ?
As2 Fe3 Fe3 125.202(16) 1_565 25_455 ?
As2 Fe3 Fe3 125.202(16) 25 25_455 ?
Fe3 Fe3 Fe3 180.0 25_565 25_455 ?
As2 Fe3 Fe3 125.203(16) . 25_465 ?
As2 Fe3 Fe3 54.798(16) 25_455 25_465 ?
As2 Fe3 Fe3 54.798(16) 1_565 25_465 ?
As2 Fe3 Fe3 125.202(16) 25 25_465 ?
Fe3 Fe3 Fe3 90.0 25_565 25_465 ?
Fe3 Fe3 Fe3 90.0 25_455 25_465 ?
As2 Fe3 Fe3 54.797(16) . 25 ?
As2 Fe3 Fe3 125.202(16) 25_455 25 ?
As2 Fe3 Fe3 125.202(16) 1_565 25 ?
As2 Fe3 Fe3 54.798(16) 25 25 ?
Fe3 Fe3 Fe3 90.0 25_565 25 ?
Fe3 Fe3 Fe3 90.0 25_455 25 ?
Fe3 Fe3 Fe3 180.0 25_465 25 ?
As2 Fe3 Sn1 82.8(3) . . ?
As2 Fe3 Sn1 64.77(13) 25_455 . ?
As2 Fe3 Sn1 168.0(3) 1_565 . ?
As2 Fe3 Sn1 64.77(13) 25 . ?
Fe3 Fe3 Sn1 118.60(17) 25_565 . ?
Fe3 Fe3 Sn1 61.40(17) 25_455 . ?
Fe3 Fe3 Sn1 118.60(17) 25_465 . ?
Fe3 Fe3 Sn1 61.40(17) 25 . ?
As2 Fe3 Sn1 64.77(13) . 25 ?
As2 Fe3 Sn1 168.0(3) 25_455 25 ?
As2 Fe3 Sn1 64.77(13) 1_565 25 ?
As2 Fe3 Sn1 82.8(3) 25 25 ?
Fe3 Fe3 Sn1 61.40(17) 25_565 25 ?
Fe3 Fe3 Sn1 118.60(17) 25_455 25 ?
Fe3 Fe3 Sn1 118.60(17) 25_465 25 ?
Fe3 Fe3 Sn1 61.40(17) 25 25 ?
Sn1 Fe3 Sn1 122.8(3) . 25 ?
As2 Fe3 Sn1 64.77(13) . 25_455 ?
As2 Fe3 Sn1 82.8(3) 25_455 25_455 ?
As2 Fe3 Sn1 64.77(13) 1_565 25_455 ?
As2 Fe3 Sn1 168.0(3) 25 25_455 ?
Fe3 Fe3 Sn1 118.60(17) 25_565 25_455 ?
Fe3 Fe3 Sn1 61.40(17) 25_455 25_455 ?
Fe3 Fe3 Sn1 61.40(17) 25_465 25_455 ?
Fe3 Fe3 Sn1 118.60(17) 25 25_455 ?
Sn1 Fe3 Sn1 122.8(3) . 25_455 ?
Sn1 Fe3 Sn1 85.2(6) 25 25_455 ?
As2 Fe3 Sn1 168.0(3) . 1_565 ?
As2 Fe3 Sn1 64.77(13) 25_455 1_565 ?
As2 Fe3 Sn1 82.8(3) 1_565 1_565 ?
As2 Fe3 Sn1 64.77(13) 25 1_565 ?
Fe3 Fe3 Sn1 61.40(17) 25_565 1_565 ?
Fe3 Fe3 Sn1 118.60(17) 25_455 1_565 ?
Fe3 Fe3 Sn1 61.40(17) 25_465 1_565 ?
Fe3 Fe3 Sn1 118.60(17) 25 1_565 ?
Sn1 Fe3 Sn1 85.2(6) . 1_565 ?
Sn1 Fe3 Sn1 122.8(3) 25 1_565 ?
Sn1 Fe3 Sn1 122.8(3) 25_455 1_565 ?
Ba1 Sn1 Sn1 0.0 . 17 ?
Ba1 Sn1 As2 104.9(4) . 25 ?
Sn1 Sn1 As2 104.9(4) 17 25 ?
Ba1 Sn1 As2 104.9(4) . 25_445 ?
Sn1 Sn1 As2 104.9(4) 17 25_445 ?
As2 Sn1 As2 150.2(8) 25 25_445 ?
Ba1 Sn1 As2 104.9(4) . 25_455 ?
Sn1 Sn1 As2 104.9(4) 17 25_455 ?
As2 Sn1 As2 86.2(2) 25 25_455 ?
As2 Sn1 As2 86.2(2) 25_445 25_455 ?
Ba1 Sn1 As2 104.9(4) . 25_545 ?
Sn1 Sn1 As2 104.9(4) 17 25_545 ?
As2 Sn1 As2 86.2(2) 25 25_545 ?
As2 Sn1 As2 86.2(2) 25_445 25_545 ?
As2 Sn1 As2 150.2(8) 25_455 25_545 ?
Ba1 Sn1 Fe3 137.4(3) . . ?
Sn1 Sn1 Fe3 137.4(3) 17 . ?
As2 Sn1 Fe3 49.3(2) 25 . ?
As2 Sn1 Fe3 105.9(6) 25_445 . ?
As2 Sn1 Fe3 49.3(2) 25_455 . ?
As2 Sn1 Fe3 105.9(6) 25_545 . ?
Ba1 Sn1 Fe3 137.4(3) . 25 ?
Sn1 Sn1 Fe3 137.4(3) 17 25 ?
As2 Sn1 Fe3 49.3(2) 25 25 ?
As2 Sn1 Fe3 105.9(6) 25_445 25 ?
As2 Sn1 Fe3 105.9(6) 25_455 25 ?
As2 Sn1 Fe3 49.3(2) 25_545 25 ?
Fe3 Sn1 Fe3 57.2(3) . 25 ?
Ba1 Sn1 Fe3 137.4(3) . 25_455 ?
Sn1 Sn1 Fe3 137.4(3) 17 25_455 ?
As2 Sn1 Fe3 105.9(6) 25 25_455 ?
As2 Sn1 Fe3 49.3(2) 25_445 25_455 ?
As2 Sn1 Fe3 49.3(2) 25_455 25_455 ?
As2 Sn1 Fe3 105.9(6) 25_545 25_455 ?
Fe3 Sn1 Fe3 57.2(3) . 25_455 ?
Fe3 Sn1 Fe3 85.2(6) 25 25_455 ?
Ba1 Sn1 Fe3 137.4(3) . 1_545 ?
Sn1 Sn1 Fe3 137.4(3) 17 1_545 ?
As2 Sn1 Fe3 105.9(6) 25 1_545 ?
As2 Sn1 Fe3 49.3(2) 25_445 1_545 ?
As2 Sn1 Fe3 105.9(6) 25_455 1_545 ?
As2 Sn1 Fe3 49.3(2) 25_545 1_545 ?
Fe3 Sn1 Fe3 85.2(6) . 1_545 ?
Fe3 Sn1 Fe3 57.2(3) 25 1_545 ?
Fe3 Sn1 Fe3 57.2(3) 25_455 1_545 ?
Ba1 Sn1 K1 72.9(3) . 1_455 ?
Sn1 Sn1 K1 72.9(3) 17 1_455 ?
As2 Sn1 K1 136.78(5) 25 1_455 ?
As2 Sn1 K1 54.72(8) 25_445 1_455 ?
As2 Sn1 K1 54.72(8) 25_455 1_455 ?
As2 Sn1 K1 136.78(5) 25_545 1_455 ?
Fe3 Sn1 K1 102.49(15) . 1_455 ?
Fe3 Sn1 K1 149.7(6) 25 1_455 ?
Fe3 Sn1 K1 64.48(4) 25_455 1_455 ?
Fe3 Sn1 K1 102.49(15) 1_545 1_455 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 Sn1 1.21(2) 17 ?
Ba1 Sn1 1.21(2) . ?
Ba1 As2 3.4077(17) 25 ?
Ba1 As2 3.4077(17) 9_444 ?
Ba1 As2 3.4077(17) 25_455 ?
Ba1 As2 3.4077(17) 25_545 ?
Ba1 As2 3.4077(17) 9_454 ?
Ba1 As2 3.4077(17) 9_544 ?
Ba1 As2 3.4077(17) 25_445 ?
Ba1 As2 3.4077(17) 9_554 ?
Ba1 Fe3 3.895(2) . ?
Ba1 Fe3 3.895(2) 25 ?
As2 Fe3 2.4202(13) 25_455 ?
As2 Fe3 2.4202(13) 1_545 ?
As2 Fe3 2.4202(13) 25 ?
As2 Fe3 2.4202(13) . ?
As2 Sn1 2.888(6) 25 ?
As2 Sn1 2.888(6) 25_445 ?
As2 Sn1 2.888(6) 25_455 ?
As2 Sn1 2.888(6) 25_545 ?
As2 Ba1 3.4077(17) 9 ?
As2 K1 3.4077(17) 9 ?
As2 K1 3.4077(17) 9_545 ?
As2 Ba1 3.4077(17) 9_455 ?
Fe3 As2 2.4202(13) 25_455 ?
Fe3 As2 2.4202(13) 1_565 ?
Fe3 As2 2.4202(13) 25 ?
Fe3 Fe3 2.7903(17) 25_565 ?
Fe3 Fe3 2.7903(17) 25_455 ?
Fe3 Fe3 2.7903(17) 25_465 ?
Fe3 Fe3 2.7903(17) 25 ?
Fe3 Sn1 2.914(16) . ?
Fe3 Sn1 2.914(16) 25 ?
Fe3 Sn1 2.914(16) 25_455 ?
Fe3 Sn1 2.914(16) 1_565 ?
Sn1 Sn1 2.43(4) 17 ?
Sn1 As2 2.888(6) 25 ?
Sn1 As2 2.888(6) 25_445 ?
Sn1 As2 2.888(6) 25_455 ?
Sn1 As2 2.888(6) 25_545 ?
Sn1 Fe3 2.914(16) 25 ?
Sn1 Fe3 2.914(16) 25_455 ?
Sn1 Fe3 2.914(16) 1_545 ?
Sn1 K1 4.128(7) 1_455 ?
